Diversity in Supramolecular Solid-State Architecture Formed by Self-Assembly of 1-(Diaminomethylene)thiourea and Aliphatic Dicarboxylic Acids
Janczak, Jan; Crystal Growth & Design 15 (2015) 5097–; doi:10.1021/acs.cgd.5b01049

data_4516449
_publ_contact_author
;
    Jan Janczak
    Institute  of Low Temperature and Structure Research 
    Polish Academy of Sciences
    P.O.Box 1410
    Okolna 2 str., 50-950 Wroc\/law
    Poland
;
_publ_section_title
;
 Diversity in Supramolecular Solid-State Architecture Formed by
 Self-Assembly of 1-(Diaminomethylene)thiourea and Aliphatic Dicarboxylic
 Acids
;
_journal_issue                   10
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              5097
_journal_paper_doi               10.1021/acs.cgd.5b01049
_journal_volume                  15
_journal_year                    2015
_chemical_formula_moiety         '2(C5 H7 O4), 2(C2 H7 N4 S)'
_chemical_formula_sum            'C14 H28 N8 O8 S2'
_chemical_formula_weight         500.56
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 108.60(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.381(2)
_cell_length_b                   16.044(3)
_cell_length_c                   14.255(3)
_cell_measurement_reflns_used    1527
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      29.16
_cell_measurement_theta_min      2.49
_cell_volume                     2250.2(9)
_computing_cell_refinement
;
Oxford Diffraction Poland (2008). CrysAlis Red, Version 171.32.6
;
_computing_data_collection
;
Oxford Diffraction Poland (2008). CrysAlis ccd, Version 171.32.6
;
_computing_data_reduction
;
Oxford Diffraction Poland (2008). CrysAlis Red, Version 171.32.6
;
_computing_molecular_graphics
;
Brandenburg & Putz (2006). Diamond 3.0. Crystal and Molecular
Structure Visualisation, University of Bonn, Germany
;
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      295(2)
_diffrn_detector_area_resol_mean '1024x1024 with blocks 2x2'
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.923
_diffrn_measurement_device_type  'KUMA KM-4 with area CCD detector'
_diffrn_measurement_method       \w-scan
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0562
_diffrn_reflns_av_sigmaI/netI    0.0931
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            27729
_diffrn_reflns_theta_full        28.00
_diffrn_reflns_theta_max         29.16
_diffrn_reflns_theta_min         2.49
_exptl_absorpt_coefficient_mu    0.295
_exptl_absorpt_correction_T_max  0.9591
_exptl_absorpt_correction_T_min  0.9301
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details
;
Oxford Diffraction Poland (2009). CrysAlis Red, Version 1.171.33.42.
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.478
_exptl_crystal_density_meas      1.47
_exptl_crystal_density_method    floatation
_exptl_crystal_description       paralLelepiped
_exptl_crystal_F_000             1056
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.17
_refine_diff_density_max         0.216
_refine_diff_density_min         -0.228
_refine_diff_density_rms         0.044
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.000
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     337
_refine_ls_number_reflns         5605
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.000
_refine_ls_R_factor_all          0.1614
_refine_ls_R_factor_gt           0.0432
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0038P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0365
_refine_ls_wR_factor_ref         0.0448
_reflns_number_gt                2937
_reflns_number_total             5605
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            cg5b01049_si_004.cif
_cod_data_source_block           2i4tglu_COMP3
_cod_original_cell_volume        2250.2(8)
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               4516449